- Nano Express
- Open Access
Facile Synthesis of Hierarchical Tin Oxide Nanoflowers with Ultra-High Methanol Gas Sensing at Low Working Temperature
Nanoscale Research Letters volume 14, Article number: 84 (2019)
In this work, the hierarchical tin oxide nanoflowers have been successfully synthesized via a simple hydrothermal method followed by calcination. The as-obtained samples were investigated as a kind of gas sensing material candidate for methanol. A series of examinations has been performed to explore the structure, morphology, element composition, and gas sensing performance of as-synthesized product. The hierarchical tin oxide nanoflowers exhibit sensitivity to 100 ppm methanol and the response is 58, which is ascribed to the hierarchical structure. The response and recovery time are 4 s and 8 s, respectively. Moreover, the as-prepared sensor has a low working temperature of 200 °C which is lower than that for other gas sensors of such type has been reported elsewhere. The excellent sensitivity of the sensor is caused by its complex phase mixture of SnO, SnO2, Sn2O3, and Sn6O4 revealed by XRD analysis. The proposed hierarchical tin oxide nanoflowers gas sensing material is promising for development of methanol gas sensor.
The as-obtained hierarchical tin oxide nanoflower (HTONF) gas sensor shows excellent gas-sensing performance at low working temperature (200 °C) and high annealing temperature (400 °C).
With the development of science and technology, methanol gas sensors have been widely applied in chemical industry. As a kind of colorless gas with a smell of ethanol, methanol can cause extremely serious health problems and environmental safety problems. For example, the central nervous system disorder and explosion would happen when the methanol concentration exceeds a threshold value.
Recently, the methanol gas sensing performance of variety of sensitive materials has been researched by a lot of researchers. For instance, Das et al. studied the gas sensing properties of the Mg+ 2:LaNiO3 thin film and obtained the response of 200–400 ppm methanol at 325 °C . Ji et al. investigated the high-performance methanol sensor based on GaN nanostructures grown on a silicon nanoporous pillar array and gained the high gas sensing performance at the operating temperature of 350 °C . Wang et al. reported methanol sensing properties of honeycomb-like SnO2 grown on a silicon nanoporous pillar array and showed the quick response properties at the operating temperature of 320 °C . Although the above scientists have made an excellent progress, the high working temperature and cost sufficiently restrict the application of sensor, which motivates us to fabricate a high methanol performance gas sensor working at low temperature and prepared via a simple and low-cost synthetic method.
SnO2 gas sensors attract attention of researchers due to their simple and low-cost synthesis method and room temperature operation. The huge improvement of gas sensing performance has been achieved by decreasing crystallite size [4, 5], doping by metal elements [6, 7], fabricating heterostructure of metal oxide [8, 9], and, especially, fabricating hierarchical structure [10, 11]. To date, a variety of gas sensors has been proposed to improve gas sensing to methanol, such as In2O3 porous nanospheres , three-dimensionally macroporous LaFeO3 , and aluminum-mesoporous silicon coplanar . However, the gas sensing properties of most of methanol gas sensors are not enough satisfactory. Therefore, the development of a kind of methanol gas sensor with high sensing properties at low working temperature by a simple method is still relevant.
In this work, we have tried to fabricate hierarchical tin oxide nanoflowers (HTONF) gas sensor to improve the gas sensing properties of sensor. We have performed a series of gas sensing examination of HTONF. And the results indicate the HTONF own excellent gas sensing performance (high sensitivity, good selectivity, rapid response and recover rates, and long stability) to methanol at low working temperature. The high gas sensing performance is caused by the hierarchical structure of the material and its phase composition, and this kind of hierarchical structure could provide many effective sites, which make the detected gas and material contact very well and extremely improve the gas sensing performance of the as-obtained materials.
Stannous chloride dehydrate (SnCl2·2H2O, 99.9%) and metyltrimethyl ammonium bromide (CTAB, 99.9%) were purchased from Sigma-Aldrich (USA). Sodium hydroxide (NaOH, 99.9%) was bought from Aladdin (China). The above chemical regents were analytical grade and were used without further purification. HTONFs were synthesized via the hydrothermal method. In brief, the solution of 2.2170 g stannous chloride dehydrate, 1.6032 g sodium hydroxide, and 0.7290 g metyltrimethyl ammonium bromide was dissolved and stirred in 35 ml distill water for 3 h. The as-obtained solution was transferred into a 50 ml Teflon-lined autoclave and heated for 5 h at 180 °C in a furnace and cooled down naturally. Then the resulting products were washed with distilled water and dried at 80 °C in a vacuum for 1 h. Finally, the as-obtained products were calcinated in a muffle furnace at 300, 400, 500, 600, and 700 °C for 3 h, and, as a result, the HTONF have been synthesized. The route of synthesis of HTONF is shown in Fig. 1.
Fabrication of Sensor
The HTONF gas sensor was fabricated as follows: firstly, the powders were mixed with some amount of distilled water to form a paste. After that, the paste was printed uniformly on a ceramic tube with a pair of gold electrodes. Then, a Ni-Cr alloy wire coil, as a kind of heater, was inserted into a ceramic tube to control the operating temperature. The sensor response was defined as a ratio Ra to Rg (Ra/Rg), where Ra and Rg are resistances of structures in air and target gas, respectively [15, 16]. The schematic structure of the gas sensor device is presented in Fig. 2.
The crystallinity and structure of HTONF were characterized by X-ray diffraction (XRD) ADX-2700D X-ray Powder Diffraction Instrument with CuKα radiation (λ = 1.15406 Å). The morphology of the samples was observed by scanning electron microscopy (FEI SKLSLM Magellan 400) and transmission electron microscopy (TEM, JEOLJEM-200FS). The specific surface area and pore size distribution of the samples were evaluated by Brunauer-Emmett-Teller (BET) model by Beijing JW-BK132F equipment. The mass changes of as-obtained HTONF powders were measured by thermal gravimetric analysis (TGA, SDT Q600, TA Instruments, USA). The CGS-8 system (chemical gas sensing, Beijing Elite Tech. Co. Ltd., China) was used to measure the gas sensing performance of samples.
Results and Discussion
The thermogravimetric analysis (TGA) curve of initial as-prepared powders is shown in Fig. 3; there are three stages of weight loss that can be distinguished. The first weight loss from 50 to 125 °C is due to the steaming of physiosorbed water molecule. The second weight loss in the range of 125–220 °C is attributed to the thermal degradation or the transformation of structure [17, 18]. The third stage lies in the temperature range 220–380 °С. And the thermogravimetric curve remains almost stable for temperatures over 400 °C.
XRD and BET Analysis
It is well known that interaction of Sn (II) salts with alkaline solutions such as NaOH leads to formation of SnOxH2O (x < 1) . So, in our case, the primary interaction of SnCl2 should correspond to the scheme:
Dehydration of Sn6O4(OH)4 leads to formation of SnO which is gradually oxidized by oxygen of air to SnO2:
At the same time, the mechanism of transformation of SnO to SnO2 (Scheme 3) is quite complex and accompanied by appearing of different metastable crystalline phases (Sn2O3, Sn3O4) when heated, that can be shown by the next schemes:
In turn, the oxidation of metallic tin by oxygen of air is accompanied with generation of SnO and following repeating of reaction (4 and 5). Analysis of literature revealed that the rate of formation of mixture oxides (Schemes 4–5) and their disproportioning depends on many factors: composition of the initial precursors and conditions of reaction for fabrication of SnO and following thermal annealing regime. As it was shown that the complete oxidation to SnO2 is usually observed at annealing temperatures over 450 °C.
From the results of XRD data (Fig. 4a), for the samples annealed at 300 °C, the three types of phases were observed: SnO2, Sn6O4(OH)4, SnO. Respectively, the simultaneous dehydration of Sn6O4(OH)4 and oxidation to SnO2 has place. In the XRD of samples annealed at 400 °C, the peaks of the phase Sn6O4(OH)4 are already absent that is in well agreement with the results of the thermogravimetric analysis (Fig. 3). At the same time, the peaks of low intensity that can be attributed to the phases SnO and Sn2O3 are observed (400 °C). In order to specify the composition of the material, we made a detailed XRD analysis (Fig. 4b). It allowed to confirm the previous analysis and shows phases SnO [17, 20,21,22,23,24,25,26,27,28,29] and Sn2O3  that were also observed in other studies. Increasing the annealing temperature to 500 °C leads to the complete oxidation of the phases consisting of Sn (II) and formation of pure SnO2. Further increasing of the temperature (600–700 °C) does not result in sufficient changes of phase composition of the samples.
The nitrogen absorption-desorption isotherms and pores size distribution curve are shown in Fig. 5. From Fig. 5a–e, it is clearly seen that the as-synthesized HTONF samples annealed at 400 °C show the biggest surface area (35.678 m2/g), which provides the biggest number of active sites and improves the gas sensitivity performance of the HTONF [30, 31]. In our opinion, the changes in specific surface area are part of a complex process of phase transformation accompanied with growth of nanostructures of different shapes such as leaves, needles, membranes, etc. [32,33,34,35] that strongly depends on conditions of synthesis process.
SEM and TEM Analysis
The morphology of the as-synthesized HTONF was investigated by scanning electron microscopy (SEM), as illustrated in Fig. 6. Figure 6c presents the SEM picture of the sample that forms flower-like morphology and shows good uniformity. Meanwhile, no other morphologies are observed in Fig. 6c, indicating that the proposed experimental procedure leads to formation of the only hierarchical nanoflower morphology of the product [36, 37]. A SEM image of an individual HTONF is shown in Fig. 6d. One can see that the HTONF is assembled with a lot of acicular-like nanosheets forming a shape of Callistephus chinensis flower.
It should be noted that the temperature of the hydrothermal synthesis sufficiently influenced on the morphology of the obtained composites. And SEM image of as-obtained HTONF annealed at different temperatures were shown in Fig. 6a–j. From this picture, it is very clearly seen that the morphologies of tin oxide materials will change when the annealing temperature is increased, and the tin oxide materials annealed at 400 °C shows the morphology similar to magnificent fractal structures. Such morphology should have specific surface area higher than other sintered disordered powder-like materials and it was confirmed by BET measurements (Fig. 5). As it was noted in , the as-obtained composite forms cubic shape with surface covered by nano-sheets at the temperature 140 °C. Thus, the temperature is the factor that obviously effects on the nucleation process and following growth of tin-containing composites. And the morphology of as-prepared materials will be changed when the calcination temperature changes.
The as-obtained HTONF were further investigated by HRTEM. The HRTEM images and corresponding SAED patterns of HTONF annealed at 300 °C and 400 °C are shown in Fig. 7a, b. From these pictures, it clearly indicated that as-synthesized HTONF samples annealed at 300 °C and 400 °C have polycrystalline structure and consist of SnO2, SnO, and Sn2O3 phases which is in agreement with the above XRD results and results of other research teams [35, 38].
Gas Sensing Properties
It is well known that gas sensing properties of metal oxide semiconductor gas sensors are highly dependent on the operating temperatures. In order to find out the optimal operating and annealing temperature, the HTONF gas sensors were investigated for different temperatures. Figure 8 shows the sensitivity of the as-synthesized HTONF gas sensor to 100 ppm methanol as a function of the operating temperature ranging from 164 to 265 °C. It can be seen that the as-prepared gas sensor based on the sample annealed at 400 °C exhibits the maximum response of 58 at 200 °C. The gas sensitivity greatly rises and reaches a maximum response when the operating temperature increases up to 200 °C, and then the gas sensitivity drastically decreases at further rising of the operating temperature. The relationship of sensitivity and operating temperatures can be explained by mechanism of gas adsorption and desorption on the surface of semiconductor metal oxide gas sensor . The chemical activity of a gas sensor is rather weak at low operating temperature, which leads to low sensitivity. The desorption rate of gas increases with growing the sensor surface temperature, and at a certain temperature it will exceed the adsorption rate that results in sensitivity drop . Therefore, 200 °C and 400 °C were defined experimentally as the optimum operating temperature for the gas sensing measurement and calcination temperature, respectively.
Table 1 indicates that the HTONF gas sensor possesses a better gas sensitivity to methanol at low working temperature compared with sensors based on other complicated structures. So, the studied hierarchical nanoflower structure would sufficiently improve the gas sensing performance of tin oxide material that can be used for fabrication of high-sensitivity low-cost methanol sensors.
To further analyze the reproducibility and long-term stability of gas sensor, the HTONF gas sensors with calcination at different temperatures were tested by carrying out eight cycles of response measurements of 100 ppm methanol, as-fabricated, and 60 days aged. As shown in Fig. 9a, the gas sensor annealed at the 400 °C presents good sensitivity and repeatability without visible changes after eight-cycle examination. The response and recovery time to 100 ppm methanol at 200 °C were about 4 s and 8 s, respectively. The gas sensibility was about 58 which means that the fabricated gas sensor has high sensitivity and repeatability. And this may be attributed to the hierarchical structure suitable for the pervasion and detecting methanol gas [41, 42]. From Fig. 9b, it is fairly observed that the as-synthesized gas sensor annealed at 400 °C shows good stability at the operating temperature of 200 °C within 60 days. The above results indicate that the HTONF gas sensor can be a good methanol detector [43, 44].
Figure 10a displays the dynamic response and recovery curves of the as-obtained sensor for different concentrations of methanol molecules ranging from 1 to 100 ppm at the 200 °C. It is obvious that the HTONF gas sensor annealed at 400 °C shows the good response and recovery performance. Moreover, the fabricated gas sensor has shown the response of 1.6 for the concentration of methanol as low as 1 ppm, demonstrating that the HTONF sensor can detect extremely low concentrations of methanol [45, 46].
In addition, the response behavior of the gas sensor to different concentrations of methanol at 200 °C is shown in Fig. 10b. It can be easily found that the sensor presents upward tendency when the concentration of methanol is increased. The gas sensitivity depends linearly on the concentrations of methanol vapor varying from 1 to 100 ppm. However, the gas sensitivity saturates when the concentration of methanol exceeds 2000 ppm. The phenomenon can be explained as follows: the methanol molecules are absorbed on the surface of the HTONF and participate in surface reaction, resulting in the rise of gas sensing. The gas sensor is saturated when the concentration of methanol exceeds a threshold value, and the gas sensitivity of the sensor shows slow growth [47, 48].
The sensor selectivity is a kind of extremely important parameter for sensors in the wide practical applications. The fabricated sensor has been additionally analyzed in terms of the selectivity. Figure 11 shows the gas sensing performance of the HTONF sensor to 100 ppm methanol, ethanol, acetone, formaldehyde, paraxylene, and dimethylformamide at 200 °C. Different gases have different chemical properties, leading to different gas sensitivities of the fabricated gas sensor [49, 50]. It is clearly seen that the gas sensitivity of the HTONF gas sensor annealed at 400 °C to 100 ppm methanol is 58 while the responses to 100 ppm ethanol, acetone, formaldehyde, paraxylene, and dimethylformamide are 19, 16, 10, 7, and 3, respectively. It is obviously seen that the HTONF gas sensor is much more sensitive to methanol compared with other studied gases demonstrating a high selectivity to methanol.
Gas Sensing Mechanism
The sensing mechanism of metal oxide gas sensors has been researched and reported in previous works [51, 52]. It was stated that gas sensor response mechanism mainly refers to the reaction between the target gas and the surface chemisorbed oxygen ions, which leads to changes in the resistance of the gas sensor. In order to understand the gas sensing mechanism for the as-obtained HTONF gas sensor, a schematic diagram of the mechanism is shown in Fig. 12. Generally, the reaction of gas sensor based on the as-prepared sample can be divided into two parts: firstly, when the HTONF are exposed to the air, oxygen molecules in air are absorbed on the surface of HTONF and create a number of chemisorbed oxygen species (O2(ads)−, O(ads)−, and O(ads)2−) by capturing free electrons in conduction band, which could extremely decrease the density of free carriers and form an electron depletion layer on the surface of HTONF. Therefore, the resistance of HTONF in air will increase (Ra) [43, 44]. The process can be explained as follows:
Secondly, when the as-obtained HTONF gas sensor is exposed to methanol gas, the chemisorbed oxygen species react with methanol and release electrons back to the conduction band. So, the electron depletion layer is reduced and the surface resistance (Rg) of HTONF is decreased. The chemical reaction can be presented as follows:
According to the Knudsen approach to diffusion in pores, the gas diffusivity is:
where r, T, and M are pore diameter, operating temperature, and molecular mass, respectively. From this formula, it can be easily concluded that higher operating temperature, bigger pores diameter, and lighter molecular mass play an important role in increasing the diffusion rate of detected gas [53, 54]. Therefore, the remarkable gas sensing properties of HTONF to methanol could be caused by the hierarchical structure. The hierarchical structure has a large surface area contributing to gas adsorption and desorption. As a result, the as-obtained HTONF gas sensor exhibits high sensitivity, quick response and recovery rates, and selectivity.
The presence of humidity in the atmosphere should decrease the methanol gas sensing performance of sensor by increasing the conductivity of the metal oxide gas sensor as it was described in . It is noticeable that the sensing behavior of the HTONF sensor to formaldehyde having molecular mass less than methanol, the lower sensitivity was observed comparing to methanol. The methanol and other alcohols contain hydroxyl group that allows its easy adsorption on surface of HTONF with chemisorbed oxygen. At the same time, the least molecular mass of the methanol in comparison with other alcohols provides its fast diffusion in pores of the fabricated HTONF increasing sensitivity of the material in accordance with the Knudsen approach (Eq. 12). In the series of studied gases, the noticeable is low sensitivity of the fabricated sensor to formaldehyde (Fig. 11). Although the formaldehyde molecule is even less than methanol one, it contains highly negative-polarized O atom that sufficiently impedes absorption of the molecule on the surface of material with chemisorbed oxygen species and consequently sensitivity of the device to that gas is low.
In light of the results obtained from XRD spectra, thermogravimetric curve, and surface area measurements, the model of sensitivity we proposed also accounts the next two reasons. The material annealed at temperatures below 450 °C includes several phases of tin oxides: SnO2, Sn2O3, and Sn3O4. These phases are responsible, by our opinion, for high sensitivity properties of the obtained structures, as it was reported by different research teams in recent publications.
The second factor is the high specific surface area of the sample 400 °C. Annealing of the samples at temperature 300 °C and 500 °C and higher results in formation of the developed surface with area value less than that of the sample annealed at 400 °C. The two described factors effect onto the sensitivity in opposite ways. And the compromise annealing temperature 400 °C resulted in simultaneously high value of the surface area and the high-sensitive tin oxides Sn2O3 and Sn3O4. It led to the highest sensitivity of the fabricated sensor based on HTONF.
In summary, hierarchical tin oxide nanoflowers for gas sensors have been synthesized via one-type hydrothermal route. A series of results indicates that the HTONF gas sensor shows high gas sensitivity, short response and recovery time, long stability, and high reproducibility. The gas response of the as-obtained gas sensor to 100 ppm methanol is about 58 and response/recovery time is about 4 s and 8 s, respectively. The excellent gas sensing performance of the HTONF sensor is attributed to the original hierarchical structure and phase composition of tin oxides. The HTONF could be a desirable candidate for applications in sensor area.
Hierarchical tin oxide nanoflowers
Scanning electron microscopy
Transmission electron microscopy
Thermal gravimetric analysis
X-ray powder diffraction Instrument
Das S, Murthy ASR, Gnanasekar KI, Jayaraman V (2018) Solution processed Mg+2:LaNiO3 thin films for effective methanol sensing. Sens Actuator B 254:526–532
Ji HF, Liu WK, Li S, Li Y, Shi ZF, Tian YT, Li XJ (2017) High-performance methanol sensor based on GaN nanostructures grown on silicon nanoporous pillar array. Sens Actuator B 250:518–524
Wang LL, Li ZJ, Luo L, Zhao CZ, Kang LP, Liu DW (2016) Methanol sensing properties of honeycomb-like SnO2 grown on silicon nanoporous pillar array. J Alloys Compd 682:170–175
Quy CT, Thai NX, Hoa ND, Le DTT, Hung CM, Duy NV, Hieu NV (2018) C2H5OH and NO2 sensing properties of ZnO nanostructures: correlation between crystal size defect level and sensing performance. RSC Adv 8:5629–5639
Tan WH, Tan JF, Li L, Dun MH, Huang XT (2017) Nanosheets-assembled hollowed-out hierarchical Co3O4 microrods for fast response/recovery gas sensor. Sens Actuator B 249:66–75
Bulemo PM, Cho HJ, Kim DH, Kim ID (2018) Facile synthesis of Pt-functionalized Meso/macroporous SnO2 hollow spheres through in situ templating with SiO2 for H2S sensors. ACS Appl Mater Interfaces 10:8183–18191
Rong Q, Zhang YM, Wang C, Zhu ZQ, Zhang J, Liu QJ (2017) A high selective methanol gas sensor based on molecular imprinted Ag-LaFeO3 fibers. Sci Rep 7:12110
Chen GH, Ji SZ, Li HD, Kang XL, Chang SJ, Wang YN, Yu GW, Lu JR et al (2015) High-energy faceted SnO (2)-coated TiO (2) Nanobelt Heterostructure for near-ambient temperature-responsive ethanol sensor. ACS Appl Mater Interfaces 7:24950–24956
Wang QJ, Kou XY, Liu C, Zhao LJ, Lin TT, Liu FM et al (2018) Hydrothermal synthesis of hierarchical CoO/SnO2 nanostructures for ethanol gas sensor. J Colloid Interface Sci 513:760–766
Shu SM, Wang MX, Yang W, Liu ST (2017) Synthesis of surface layered hierarchical octahedral-like structured Zn 2 SnO4/SnO2 with excellent sensing properties toward HCHO. Sens Actuator B 243:1171–1180
Zhang R, Zhou TT, Wang LL, Zhang T (2018) Metal-organic frameworks-derived hierarchical Co3O4 structures as efficient sensing materials for acetone detection. ACS Appl Mater Interfaces 10:9765–9773
Han D, Song P, Zhang S, Zhang HH, Xu Q, Wang Q (2015) Enhanced methanol gas-sensing performance of Ce-doped In2O3 porous nanospheres prepared by hydrothermal method. Sens Actuator B 216:488–496
Qin J, Cui ZD, Yang XJ, Zhu SL, Li ZY, Liang YQ (2015) Synthesis of three-dimensionally ordered macroporous LaFeO3 with enhanced methanol gas sensing properties. Sens Actuator B 209:706–713
Khardani M, Bouaïcha M, Boujmil MF, Bessaïs B (2010) Aluminum-mesoporous silicon coplanar type structure for methanol gas sensing. Micropor Mesopor Mater 135:9–12
Ji FX, Ren XP, Zheng XY, Liu YC, Pang LQ, Jiang JX, Liu SZ (2016) 2D-MoO3 nanosheets for superior gas sensors. Nanoscale 8:8696–8703
Zhang ZY, Zou XM, Xu L, Liao L, Liu W, Ho J, Xiao X, Jiang CZ, Li J (2015) Hydrogen gas sensor based on metal oxide nanoparticles decorated graphene transistor. Nanoscale 7:10078–10084
Feng LD, Huang XJ, Choi YK (2006) Dynamic determination of domestic liquefied petroleum gas down to several ppm levels using a Sr-doped SnO2 thick film gas sensor. Microchim Acta 156:245–251
Mali SS, Patil JV, Kim H, Hong CK (2018) Synthesis of SnO2 nanofibers and nanobelts electron transporting layer for efficient perovskite solar cells. Nanoscale 10:8275–8284
Holleman AF, Wiberg E, Tin FA (2001) Holleman - Wiberg Inorganic Chemistry. Academic Press, New-York. p. 904
Yu H, Yang TY, Wang ZY, Li ZF, Xiao BX, Zhao Q, Zhang M (2017) Facile synthesis cedar-like SnO2 hierarchical micro-nanostructures with improved formaldehyde gas sensing characteristics. J Alloys Compd 724:121–129
Yang DJ, Kamienchick I, Youn DY, Rothschild A, Kim ID (2010) Ultrasensitive and highly selective gas sensors based on electrospun SnO2 nanofibers modified by Pd loading. Adv Funct Mater 20:4258–4264
Murken VG, Tromel M (1973) Uber das bei der Disproportionierung von SnO entstehende Zinnoxid, Sn203. Z anorg. Allg Chem 397:117–126
Yu H, Yang TY, Wang ZY, Li ZF, Zhao Q, Zhang MZ (2018) p-N heterostructural sensor with SnO-SnO2 for fast NO2 sensing response properties at room temperature. Sens Actuator B 258:517–526
Zhang YQ, Li D, Qin LG, Zhao PL, Liu FM, Chuai XH, Sun P et al (2018) Preparation and gas sensing properties of hierarchical leaf-like SnO2 materials. Sens Actuator B 255:2944–2951
Wang Q, Yao N, An DM, Li Y, Zou YL, Lian XX, Tong XQ (2016) Enhanced gas sensing properties of hierarchical SnO2 nanoflower assembled from nanorods via a one-pot template- free hydrothermal method. Ceram Int 42:15889–15896
Suman PH, Longo E, Orlandi MO (2014) Controlled synthesis of layered Sn3O4 nanobelts by carbothermal reduction method and their gas sensor properties. J Nanosci Nanotechnol 14:6662–6668
He YH, Li DZ, Chen J, Shao Y, Xian JJ, Zheng XZ, Wang P (2014) Sn3O4: A novel heterovalent-tin photocatalyst with hierarchical 3D nanostructures under visible light. RSC Adv 4:1266–1269
Balgude SD, Sethi YA, Kale BB, Munirathnam NR, Amalnerkar DP, Adhyapak PV, He Y et al (2014) Sn3O4: a novel heterovalent-tin photocatalyst with hierarchical 3D nanostructures under visible light. RSC Adv 4:1266–1269
Patil JV, Kim H, Hong CK (2018) Synthesis of SnO2 nanofibers and nanobelts electron transporting layer for efficient perovskite solar cells. Nanoscale 10:8275–8284
Stanoiu A, Simion CE, Sackmann A, Baibarac M, Florea OG et al (2018) Networked mesoporous SnO2 nanostructures templated by Brij ® 35 with enhanced H2S selective performance. Micropor Mesopor Mater 270:93–101
Yang FC, Guo ZG (2016) Tuning SnO2 architectures with unitary or composite microstructure for the application of gas sensors. J Colloid Interface Sci 462:140–147
Zhao CH, Gong HM, Lan WZ, Xu H, Liu S, Wang F et al (2018) Facile synthesis of SnO2 hierarchical porous nanosheets from graphene oxide sacrificial scaffolds for high-performance gas sensor. Sens Actuator B 258:492–500
Liu XH, Ma TT, Xu YS, Sun L, Zheng LL, Schmidt OG, Zhang J (2018) Rolled-up SnO2 nanomembranes: a new platform for efficient gas sensors. Sens Actuator B 264:92–99
Zou YH, Chen S, Sun J, Liu JQ, Che YK, Liu XH, Zhang J, Yang DJ (2017) Highly efficient gas sensor using a hollow SnO2 microfiber for triethylamine detection. ACS Sens 2:897–902
L XY, Peng K, Dou YW, Chen JS, Zhang Y, An G (2018) Facile synthesis of wormhole-like mesoporous tin oxide via evaporation induced self-assembly and the enhanced gas-sensing properties. Nanoscale Res Lett 13:14
Hu J, Wang T, Wang YJ, Huang D, He GL, Han YT, Hu NT et al (2018) Enhanced formaldehyde detection based on Ni doping of SnO2 nanoparticles by one-step synthesis. Sens Actuator B 263:120–128
Tammanoon N, Wisitsoraat A, Phokharatkul D, Tuantranont A, Phanichphant S, Yordsri V, Liewhiran C (2018) Highly sensitive acetone sensors based on flame-spray-made La2O3 -doped SnO2 nanoparticulate thick films. Sens Actuator B 262:245–262
Cheng DL, Hou XX, Wen HJ, Wang Y, Wang HL, L XJ, Lu HX et al (2010) The enhanced alcohol-sensing response ultrathin WO3 nanoplates. Nanotechnology 21:035501
Ma YH, Lu Y, Gou HT, Zhang WX, Yan SH, Xu XL (2018) Octahedral NiFe2O4 for high-performance gas sensor with low working temperature. Ceram Int 44:2620–2625
Xu SP, Zhao HP, Xu Y, Xu R, Lei Y (2018) Carrier mobility-dominated gas sensing: a room-temperature gas-sensing mode for SnO2 nanorod array sensors. ACS Appl Mater Interfaces 10:13895–13902
Tan JF, Dun MH, Li L, Zhao JY, Tan WH, Lin ZD, Huang XT (2017) Synthesis of hollow and hollowed-out Co3O4 microspheres assembled by porous ultrathin nanosheets for ethanol gas sensors: responding and recovering in one second. Sens Actuator B 249:44–52
Xiong Y, Zhu ZY, Ding DG, Lu WB, Xue QZ (2018) Multi-shelled ZnCo2O4 yolk-shell spheres for high-performance acetone gas sensor. Appl Surf Sci 443:114–121
Ma L, Ma SY, Shen XF, Wang TT, Jiang XH, Chen Q, Qiang Z et al (2018) PrFeO3 hollow nanofibers as a highly efficient gas sensor for acetone detection. Sens Actuator B 255:2546–2554
Wang JQ, Li ZJ, Zhang S, Yan SN, Cao BB, Wang ZG, Fu YQ (2018) Enhanced NH3 gas-sensing performance of silica modified CeO2 nanostructure based sensors. Sens Actuator B 255:862–870
Li YX, Zu BY, Guo YN, Li K, Zeng HB, Dou XC (2016) Surface superoxide complex defects-boosted ultrasensitive ppb-level NO2 gas sensors. Small 12:1420–1424
Shingange K, Tshabalala ZP, Ntwaeaborwa OM, Motaung DE, Mhlongo GH (2016) Highly selective NH3 gas sensor based on au loaded ZnO nanostructures prepared using microwave-assisted method. J Colloid Interface Sci 479:127–138
Li ZJ, Wang JQ, Zhang S, Yan SN, Cao BB, Shen WZ, Wang ZG, Fu YQ (2018) Highly sensitive NH3 gas sensor based on the porous Ce0.94Zr0.06O2 nano-sheets with ppb level detection limit. J Alloys Compd 742:712–720
Liu X, Chen N, Han BQ, Xiao XC, Chen G, Djerdj I, Wang YD (2015) Nanoparticle cluster gas sensor: Pt activated SnO2 nanoparticles for NH3 detection with ultrahigh sensitivity. Nanoscale 7:14872–14880
Chen Z, Umar A, Wang SW, Wang Y, Tian T, Shang Y, Fan YZ, Qi Q et al (2015) Supramolecular fabrication of multilevel graphene-based gas sensors with high NO2 sensibility. Nanoscale 7:10259–10266
Rai P, Yoon JW, Jeong HM, Hwang SJ, Kwak CH, Lee JH (2014) Design of highly sensitive and selective Au@NiO yolk-shell nanoreactors for gas sensor applications. Nanoscale 6:8292–8299
Liu XH, Ma TT, Pinna N, Zhang J (2017) Two-dimensional nanostructured materials for gas sensing. Adv Funct Mater 27:1702168
Wang Q, Yao N, An DM, Li Y, Zou YL, Lian XX, Tong XQ (2016) Enhanced gas sensing properties of hierarchical SnO2 nanoflower assembled from nanorods via a one-pot template-free hydrothermal method. Ceram Int 42:15889–15896
Simion CE, Somacescu S, Teodorescu VS, Osiceanu P, Stanoiu A (2018) H2S sensing mechanism of SnO2-CuWO4 operated under pulsed temperature modulation. Sens Actuator B 259:258–268
Yang HM, Ma SY, Yang GJ, Jin WX, Wang TT, Jiang XH, Li WQ (2016) High sensitive and low concentration detection of methanol by a gas sensor based on one-step synthesis α-Fe2O3 hollow spheres. Mater Lett 169:73–76
Kumar A, Kumar M, Kumar R, Singh R, Prasad B, Kumar D (2019) Numerical model for the chemical adsorption of oxygen and reducing gas molecules in presence of humidity on the surface of semiconductor metal oxide for gas sensors applications. Mat Sci Semicon Proc 90:236–244
This work has been supported by the national long-term project [no. WQ20142200205] of Thousand Talents Plan of Bureau of Foreign Experts Affairs of the People’s Republic of China.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Song, L., Lukianov, A., Butenko, D. et al. Facile Synthesis of Hierarchical Tin Oxide Nanoflowers with Ultra-High Methanol Gas Sensing at Low Working Temperature. Nanoscale Res Lett 14, 84 (2019) doi:10.1186/s11671-019-2911-4
- Hierarchical tin oxide nanoflowers
- Hydrothermal method
- Gas sensor